Germanium (Ge) has played a key role in silicon photonics as an enabling material for datacom applications. Indeed, the unique properties of Ge have been leveraged to develop high performance integrated photodectors, which are now mature devices. Ge is also very useful for the achievement of compact modulators and monolithically integrated laser sources on silicon. Interestingly, research efforts in these domains also put forward the current revolution of mid-IR photonics. Ge and Ge-based alloys also present strong advantages for mid-infrared photonic platform such as the extension of the transparency window for these materials, which can operate at wavelengths beyond 8 μm. Different platforms have been proposed to take benefit from the broad transparency of Ge up to 15 μm, and the main passive building blocks are now being developed. In this review, we will present the most relevant Ge-based platforms reported so far that have led to the demonstration of several passive and active building blocks for mid-IR photonics. Seminal works on mid-IR optical sensing using integrated platforms will also be reviewed.
Today, silicon photonics is a mature technology for integrated photonics, which benefits from a reliable and high-volume fabrication to offer high performance, low cost and compact photonic circuits. Among the different materials available in silicon photonics, germanium (Ge), silicon-germanium (SiGe) and germanium-tin (GeSn) play a key role at different maturity level in establishing essential functionalities required for a photonic integrated platform. First applications of silicon photonics were dedicated to Datacom in the near-InfraRed (near-IR) wavelength range. While Ge photodetectors have been considered for a long time as a key component in the receiver part, the small energy difference between the direct and the indirect band gap energy of Ge also makes it an ideal candidate to develop compact electro-absorption modulators and to envision on-chip monolithically integrated lasers. Besides the demonstration of efficient devices, an in-depth understanding of the properties of Ge, SiGe and GeSn is required to properly and finely tune several parameters such as the concentration of Ge or Sn in the alloys, doping or lattice strain.
More recently, it appeared that Ge also presents distinctive advantages for mid-infrared (mid-IR) photonics owing to its wide transparency window up to 15 μm and a strong non-linear refractive index. Main foreseen applications stand for the development of new mid-IR spectroscopic sensing systems that need to be portable and cost-effective, or free space optical communications for wavelengths beyond 8 μm. Previous works at telecom wavelength paved the way towards a new playground for photonic researchers as manifold engineering possibilities are now opened using Ge, SiGe and GeSn for both passive and active functions.
In this context, we will review the development of Ge-based photonic integrated circuits. For near-IR photonics applications, previous review papers have been devoted to monolithic integrated Ge-on-Si active photonics , , , . Thus, we will just recall hereafter the main motivations for the development of Ge-based devices and summarize major results. Interestingly, we will see how these works put forward the current revolution of mid-IR photonics . Indeed Ge is a unique candidate for extending the operating wavelength of Group IV-based photonic integrated circuits beyond 8 μm. The different integrated platforms used up to now will be presented, emphasizing on the development of passive functions such as cavities or spectrometers and on preliminary sensing demonstrations. Current demonstrations have already been reported up to 8.5 μm, typically for the moment, in a rapidly growing research field with a strong potential to reach wavelengths up to 15 μm. In parallel, state-of-the-art Si-based mid-IR photonics circuits can be found in recent review papers , , . Finally, the progress towards integrated active devices such as a monolithically integrated source, the modulator and the photodetector will be presented and future perspectives opened by these works will be drawn. The fine comprehension of a myriad of physical effects including the non-linear optical effect, the free-carrier plasma effect or intersubband transitions in quantum systems can thus lay the foundations for the implementation of efficient mid-IR chip-scale systems with an unprecedented number of applications such as absorption spectroscopy for chemical or biological sensing, environmental monitoring, datacom or free-space optical communications, to name a few.
2 Ge-based near-IR photonic integrated circuits
The investigation of Silicon-on-Insulator (SOI) as a platform for photonic integration dated back to 1990s with the first demonstrations of low-loss propagation in the near-IR range . The large refractive index contrast between silicon (Si) and silicon dioxide (SiO2) provides a strong light confinement, leading to ultra-compact waveguides such as nanowires with transversal dimensions of a few hundreds of nanometers with tight bend radius. Up to now, the development of silicon photonics has been mainly driven by telecom and datacom applications, requiring fiber-to-chip light coupling, on-chip routing, wavelength filtering and polarization management. All of these passive functions have been successfully demonstrated and miniaturized based on the SOI platform. However, transceivers also require the on-chip integration of active photonic functionalities such as light emitter, modulator and photodetector (Figure 1). Si is an indirect bandgap material, having a bandgap energy of 1.1 eV. It thus exhibits poor emission and detection properties in the near-IR wavelength (1.3–1.55 μm). This frequency window is used for telecom applications due to the dispersion characteristics and low-propagation losses in optical fibers at these wavelengths. Thus, different strategies have been used to develop active devices on SOI platform, mainly based on monolithic or heterogeneous integration of other materials. Rapidly, Ge appeared to be a material of choice for monolithic integration, due to its compatibility with Si CMOS technology. Furthermore, its direct bandgap energy of 0.8 eV is compatible with near-IR light absorption. Ge photodetectors have thus been developed since the late 1990s , , , . To deal with the lattice mismatch between Si and Ge, a two-step growth process has been proposed and largely adopted, in which a thin layer is first epitaxially grown at low temperature to relax the strain between Si and Ge and confine dislocations at the two material interface. Then, in a second step, a thick Ge layer can be grown at high temperature, allowing for the achievement of an active material with a good crystalline quality. Post-grown temperature annealing can also be used. Based on this approach, Ge photodetectors rapidly achieved outstanding performances. High responsivity, high speed operation and low dark current have been demonstrated in different configurations , , , , , , , , , , , , , , . Ge photodetectors are now considered to be a mature device, available in multi-project-wafer (MPW) platforms [https://mycmp.fr/IMG/pdf/overwier_cea_leti_ic_si310-phmp2m_june2017.pdf, http://www.aimphotonics.com/pdk, https://www.imec-int.com/en/silicon-photonic-ICs-prototyping, https://www.a-star.edu.sg/ime/SERVICES/R-D-Fab/silicon_photonics_multi-projects-wafer] and also in industrial foundries , https://www.globalfoundries.com/technology-solutions/silicon-photonics].
In parallel with the development of Ge photodetectors, an extensive number of works has been devoted to silicon-based optical modulators. Phase modulation by free-carrier concentration variation is used to achieve high-speed modulation in silicon, and many different configurations have been proposed to optimize the typically trade-offs between efficiency, loss and speed. Electrical structures such as PN, PIN, PIPIN diodes or MOS capacitors have been integrated in SOI waveguides to achieve carrier injection, depletion or accumulation. An overview of the early evolution of Si modulator can be found in Ref. . State-of-the-art silicon on-off keying (OOK) modulators are currently reaching 50-Gb/s operation , , ,  while advanced multi-level modulation formats such as n-level pulse amplitude modulation (PAM-n), quadrature phase-shift keying (QPSK), or even 16-level quadrature amplitude modulation (16-QAM) allow to increase transmission data rate up to 224 Gb/s , , , , , . Interestingly, while most of the reported works have been carried out in the conventional communication band (C-band) centered around 1550 nm, silicon photonics systems are also highly attractive for short-reach applications such as intra-data-center communications. Those are typically located in the original communication window (O-band), around the wavelength of 1310 nm, to benefit from negligible chromatic dispersion of standard optical fibers. Despite the lower free-carrier dispersion effect at this wavelength in comparison with the C-band, high-performance devices have been demonstrated, showing 50-Gbit/s OOK modulation  or low-voltage operation . Developing higher-order modulation formats in the O-band is also receiving significant amount of research attention , , , .
Like Ge photodetectors, Si modulators are currently mature devices available for applications. However for some specific applications, for instance short-reach communications, the power consumption of the modulator is recognized as a key metric that has to be minimized to overpass current electrical-based interconnects. It has thus been evaluated that to effectively replace copper wire for chip-to-chip or on-chip communications, the power consumption of the optical modulator has to be below 100 fJ/bit . Silicon modulator based on carrier concentration variations typically requires the use of an active region with a length of a few millimeters, altogether with voltages of a few volts. The energy consumption required to charge/discharge the corresponding capacitance is typically of a few pJ/bit. Resonant structures can take benefit from a nonlinear transfer function to reduce the active region surface, the price to pay being a reduced optical bandwidth. Electroabsorption can be used to overcome this problem and to provide compact (<100 μm) and low power consumption (<100 fJ/bit) optical modulator. Despite being an indirect bandgap material, the small difference between the direct and the indirect bandgap energy of Ge allows the achievement of strong electroabsorption at its direct bandgap energy. Ge or SiGe Franz-Keldysh modulator monolithically integrated on silicon have been reported since 2008 , and followed by different demonstrations , , . Recent works have shown that these SiGe modulators are now reaching a strong maturity towards applications in telecommunications field , , , . Electroabsorption using Ge/SiGe Multiple Quantum Wells (MQW) has also been studied, with a first demonstration in 2005 . As a main advantage in comparison with Franz-Keldysh effect, the absorption band-edge of the QW structure can be tuned to achieve modulation at 1.55 ,  or 1.3 μm ,  wavelengths, i.e. in the C- or O-band of communications. Strain compensated Ge/SiGe QW can be grown on Ge-rich SiGe virtual substrates, obtained by the growth of a thick (typically 10 μm) graded buffer from Si to Ge-rich SiGe layer, followed by a 2-μm-thick Ge-rich SiGe layer. Good quality of Ge/SiGe QW was obtained, with a reduced width of the excitonic absorption peak of about 6 meV . A review of the early achievements towards photonic integrated circuits based on Ge/SiGe QW can be found in Ref. . More recently, attention has been dedicated to the possibility to achieve phase modulation by QCSE . A giant electro-optic effect has already been demonstrated in coupled quantum-well structures . As a main challenge, the integration of Ge/SiGeQWs with SOI waveguides remains the main limiting factor to develop silicon photonics transceivers based on Ge/SiGe QW , , , . As an alternative path, it was proposed to use Ge-rich SiGe virtual substrates as a passive waveguide, allowing the demonstration of an on-chip transmission link using Ge/SiGe QW modulator and photodetector grown on Si substrate . This new platform was further explored, and the possibility to achieve tight bends, MMIs and Mach-Zehnder interferometers was demonstrated .
The possibility to use the direct gap transition of Ge and SiGe alloys has also opened an exciting research field towards the monolithic integration of light sources on photonic integrated circuits , , , , , . The realization of a Ge-based laser source requires band engineering to tailor the Ge properties accordingly, targeting an efficient direct band gap emission. An alternative approach has been proposed, using GeSn alloys to achieve a direct band gap material. GeSn laser has thus been demonstrated both optically and electrically pumped , , . It can be noted that increasing Sn concentration in the alloy also creates a reduction of the bandgap energy, shifting the operation wavelength towards 2–3 μm, opening a perspective, for instance, in the use of new communications wavelengths.
3 Ge-based mid-IR photonic integrated circuits: passive circuits
During the last 15 years, Ge-based active devices have been developed to complement Si passive photonics circuits. This evolution, which was first driven by Telecom and Datacom applications in the near-IR, later became preclude of promising new perspectives using longer wavelengths in the mid-IR range. Figure 2 shows material transparency windows with optical loss below 2 dB/cm .
While Si is transparent up to 8 μm wavelength, the strong absorption of SiO2 is expected to limit the operating wavelength range of conventional SOI waveguides beyond 4 μm. However, different strategies have appeared recently such as a proper design of SOI waveguide to limit the overlap of the optical mode with the lower silicon dioxide cladding . Other options rely on the combination of Si membrane engineered by sub-wavelength grating nano-structuration to achieve air-cladded Si waveguides , the use of Si nanopillars , or Si on Sapphire . The state-of-the-art Si-based mid-IR devices such as waveguides, sources, modulators or photodetectors can be found in recent review papers , , .
In parallel with the development of Si-based mid-IR photonic circuits, Ge is a prime candidate to extend the operating wavelength of Group IV-based photonic integrated circuits beyond 8 μm, potentially up to 15 μm , . Furthermore, Ge benefits from a strong third-order nonlinearity which can also be advantageously exploited for the development of active devices . In the last years, the development of photonic platforms dedicated to longer mid-IR wavelengths has witnessed a burst of research activity, mainly based on Ge or SiGe alloys. We will first review the different Ge-based photonic platforms. In the different cases, the characterization of the waveguide propagation losses is the starting point to evaluate the potential usefulness of each platform. Then, passive photonic devices have been developed to create a set of building blocks that can be further combined to form future mid-IR photonic integrated circuits. Among all, on-chip resonators are one of the key building blocks to be exploited in the mid-IR spectral range, for the development of on-chip sensing, spectroscopy, as well as nonlinear optical functionalities. In the following, we will review the different proof-of-concepts towards molecular sensing, before focusing on the active devices such as optical sources or modulators.
3.1 Different waveguide platforms
Initial works used Germanium-on-Silicon (GOS) waveguides. Losses of 2.5 dB/cm have been obtained at 5.8 μm wavelength . Mid-IR wavelength (de)multiplexers based on planar concave gratings (PCGs)  and Arrayed Waveguide Grating (AWG) Multiplexers  have been demonstrated, providing an operation in the 5-μm wavelength range. The GOS platform is widely used in photonics research presently and many impressive achievements have been performed even on active building blocks as will be shown later. The lowest propagation loss on that platform reported so far had a loss of only 0.6 dB/cm at 3.8 μm wavelength . However, the silicon bottom cladding is expected to limit the device operation to wavelengths shorter than 8 μm. Recent work reported propagation from 7.5 to 8.5 μm wavelength. A minimum value of 2.5 dB/cm at λ ~7.5 μm was obtained; however, losses rapidly increased for longer wavelengths up to 20 dB/cm . Optical and nonlinear properties of GOS waveguides have also been studied theoretically to define waveguide design guidelines for several applications . GOS cavities have been developed around 3.8 μm wavelength, based on racetrack resonators .
In parallel with the GOS platform, Ge-on-SOI could present some advantages, especially in terms of thermal and electrical isolation due to the underlying SiO2 buffer. However, optical absorption in the buried oxide buffer can limit the transparency range of the Ge-on-SOI platform beyond 3.6 μm wavelength. Losses of 8 dB/cm have been achieved for 0.85-μm-thick Ge core at 3.682 μm wavelength , while comparable values of 7 dB/cm have been reported previously in the wavelength range of 5.25–5.35 μm . Thermo-optic phase shifters have also been developed  and used to achieve thermally tunable racetrack resonators in the 5 μm wavelength range .
Ge-On-Insulator (GeOI) and Ge-on Silicon Nitride (SiN) have also been proposed to benefit from larger index contrast between Ge (n=4) and SiO2 (n=1.4) or SiNx (n=1.9). Propagation loss was found to be 1.4 dB/mm for GeOI rib waveguides at 2 μm wavelength, while negligible bend loss was obtained even with a 5-μm bend radius, owing to the strong optical confinement in the GeOI structure . Ge-on-SiN should benefit from a transparent cladding up to about 7.5 μm wavelength. At the wavelength of 3.8 μm, the Ge-on-SiN waveguide has a propagation loss of 3.3 dB/cm and a bend loss of 0.14 dB/bend for a radius of 5 μm .
Ge membrane is an ultimate way to take benefit from the wide transparency of Ge, without any limitation from cladding absorption. Resonators have been demonstrated around 2 μm wavelength based on air-cladded Ge membranes. Photonic crystal cavity has offered a moderate Q factor of 200 , while more recently a loaded Q-factor of ~57,000 has been achieved around 2 μm wavelength, using an air-cladding Ge micro-ring resonator .
Fiber-to-chip grating couplers have been demonstrated for the different waveguide platforms, first at 3.8 μm wavelength for GOS substrate  and then at 5.2 μm wavelength for both GOS and Ge-on-SOI platforms . In the last case, −5 dB efficiency with a 3-dB bandwidth of 100 nm was obtained for GOS grating couplers, while −4 dB efficiency with a 3-dB bandwidth of 180 nm was achieved for Ge-on-SOI case. Coupling into suspended Ge membrane was also demonstrated using focusing subwavelength grating coupler at a wavelength of 2.37 μm .
In parallel with pure Ge-based waveguides, the use of SiGe alloys presents the advantage to allow fine tuning of the waveguide properties such as refractive index and dispersion. Graded SiGe/Si waveguides have been investigated first. In this case, the core itself of the waveguide was graded, with a Ge concentration from 0% to 40% and losses as low as 1 dB/cm at λ=4.5 μm and 2 dB/cm at 7.4 μm was thus demonstrated . Passive functions such as AWG multiplexer have then been obtained, operating at 4.5 μm . Si0.6Ge0.4 waveguide on Si substrate has also been used to define dispersion engineered strip waveguides . Minimal losses of 0.5 dB/cm at 4.75 μm was obtained .
On another hand, we have recently proposed Ge-rich Si1−xGex alloys on graded Si1−xGex layers as an alternative approach for mid-IR integrated photonics. One of the relevant features of these waveguides is their expected wide transparency window, which could potentially extend up to λ=15 μm, as the refractive index gradient allows to push the optical mode far from the Si substrate.
Propagation losses lower than 2 dB/cm were first obtained at 4.6 μm wavelength , while losses of 2–3 dB/cm were then demonstrated between 5.5 and 8.5 μm wavelength . Broadband Mach-Zehnder interferometers have been demonstrated, working in both quasi-TE and TM polarizations . Interestingly, these structures also allow to finely tune the refractive index profile, permitting an efficient tailoring of the waveguide properties such as mode confinement and dispersion. An optimal design was investigated and a graded 6-μm-thick Si1−xGex stack was defined as an attractive platform to develop mid-IR nonlinear approaches requiring broadband dispersion engineering . Additionally wideband and polarization-insensitive waveguides can also be designed by optimizing waveguide dimensions, opening new perspectives for mid-IR free-space communications . First resonators on this platform, based on Fabry-Perot cavity, demonstrated a Q-factor of more than 1200 at 8.4 μm wavelength .
So far, first generations of Ge-based waveguides have already exhibited interesting properties up to 8.5 μm wavelength as summarized in Figure 3. Waveguide performance is continuously improving, and their operation wavelength is rapidly increasing towards 15 μm which is the theoretical maximum that can be expected. Efforts have also been devoted to build basic elements for further complex functionalities within the Ge platform.
3.2 Sensing demonstrations
In parallel to the development of passive devices based on the Ge platform, the potential for sensing is also being evaluated by several research groups. Optical biosensors are generally based on the sensitivity of optical structures to changes in the surrounding materials to detect the presence of molecules. Refractive index variations can then be detected using Si- or Ge-based photonics devices, such as resonators , photonic crystals  or PIN photodetectors . Most of these works are reported around 1.5 μm wavelength because of the availability of test equipments in this wavelength range. On another side, by using mid-IR integrated photonics, absorption spectroscopy can rely on the unique absorption characteristics in the fingerprint region to unambiguously identify different molecules, without the need for waveguide functionalization. The monitoring of the absorption of the evanescent component of mid-IR propagating guided modes to probe surrounding cladding environments is illustrated in Figure 4A and B. This method has been reported on different material platforms such as chalcogenide ,  or silicon . This method has also been used with Ge-based photonic integrated circuits. A Ge strip waveguide on a Si substrate, integrated with a microfluidic chip, has been used to detect cocaine in tetrachloroethylene (PCE) solutions. The demonstration was done at 5.8 μm wavelength, and small concentrations of 100 μg/ml have been successfully detected . This technique has also been explored in Ge-rich graded SiGe waveguides. The measurement of the absorption of a standalone photoresist spin-coated onto spiral Ge-rich SiGe waveguides allowed us to identify a particular optical loss characteristic within the spectral window of 5.2–7 μm and to correlate it with the inherent photoresist absorption. Based on this result, the ability of this platform to sense small concentrations of methane gas has been discussed .
Plasmonics is generally known as a way to enhance sources, sensors and detectors for applications in chemical sensing or thermal imaging. Surface plasmons can be used to confine the optical field at the surface and to strengthen the interaction between the material to be detected and the optical beam , . The challenge of mid-IR plasmonics is to propose cost-effective, compact and reliable platforms. In this context, the implementation of heavily doped Ge films is interesting as it possesses plasma frequencies in the mid-infrared range. Mid-IR plasmonics sensing using antenna made of heavily doped Ge has thus been proposed to take advantage of the CMOS platform to revolutionize plasmonic sensors usually based on gold. Detailed study of the dielectric function and the losses of heavily doped Ge in the mid-IR has been reported . Among the key challenges, increasing the doping concentration up to a value approaching 1020 cm−3 over uniform doping profile of the order of 300–500 nm would be desirable to cover the whole fingerprint region. A combination of in situ doping and excimer laser annealing has been used to improve the activation of phosphorous in germanium. An activated n-doping concentration of 8.8×1019 cm−3 was used . In terms of sensing demonstration, up to 2 orders of magnitude signal enhancement for molecules located in the heavily doped Ge antenna hot spots compared to those located on a bare silicon substrate has been obtained using an experiment schematically illustrated in Figure 4C and D . The detection and amplification of molecular absorption lines from a mustard gas simulant was also demonstrated at 14 μm wavelength .
GeSn alloys present also some interest for plasmonics sensing. Compared to Ge, GeSn alloys offer an additional benefit of lower conductivity effective mass and, thus, higher plasma frequency. Highly doped Ge0.95Sn0.05 films have been characterized by ellipsometric tools to evaluate their suitability as plasmonic materials in the IR wavelength range. It was demonstrated that n-type doped Ge0.95Sn0.05 exhibits metallic behavior at wavelengths larger than 6.4 μm, thus making the material potentially suitable for plasmonic applications even at wavelengths below 10 μm .
All these demonstrations, using absorption of the evanescent field of propagating guided modes or surface plasmon enhancement, pave the way towards the demonstration of compact, portable, label-free and highly sensitive photonic integrated sensors based on Ge mid-IR photonics circuits.
4 Ge-based mid-IR photonic integrated circuits: active building blocs
Besides the development of waveguide, resonators or sensors, the successful development of active devices to manipulate light and convert signals from electrical to optical domain can put the Ge-based platforms at the first level for future mid-IR photonics systems.
4.1 Non-linear optics in Ge and SiGe
Lots of works as well as previous review papers have been dedicated to non-linear photonics based on Si and Ge  and to mid-IR integrated photonics on Si . We have thus chosen to recall the main motivations and to focus on recent works using non-linear optics (NLO) in Ge and SiGe platform in the mid-IR.
Both Si and Ge exhibit strong third-order NLO coefficients while two-photon absorption (TPA), which is known to limit the efficiency of nonlinearities, vanishes in the mid-IR , . In terms of SiGe alloys, the properties of both Si-rich and Ge-rich waveguides have been investigated. The NLO response of Si0.6Ge0.4 waveguides has been investigated from 3.25 to 4.75 μm using picosecond optical pulses, allowing the measurement of three- and four-photon absorption coefficients as well as the Kerr nonlinear refractive index . Third-order nonlinear experimental characterizations of Si1−xGex waveguides have also been reported at a wavelength of 1580 nm for x=0.7, 0.8 and 0.9, and extrapolated in the mid-IR .
Furthermore, numerical simulations have shown that octave spanning nonlinear applications, including on-chip supercontinuum generation, ultrashort pulse compression and mode-locked wideband frequency comb generation based on micro-resonators require dispersion-flattened waveguides . Nonlinear characterizations and numerical simulations are particularly interesting as they provide insights for the design of nonlinear integrated optical based devices .
As a fundamental NLO-based device, supercontinuum generation is a way to achieve on-chip wideband source. This relies on self-phase modulation due to Kerr effect. Ge-on-Si waveguides have been designed with flat and low dispersion profile, ranging from 3 up to 11 μm. Numerical simulations have shown that such waveguide enables the generation of coherent supercontinuum in a spectral range from 2 to 12 μm . Similarly, graded-index SiGe waveguides have been engineered, allowing for broadband tight modal confinement and flat anomalous dispersion for the perspective of supercontinuum generation .
In terms of experimental demonstrations, supercontinuum has been obtained from 1.45 to 2.79 μm in a graded SiGe waveguide  and from 3 to 8.5 μm in a Si0.6Ge0.4/Si waveguide . Interestingly, an average power of more than 10 mW on-chip was obtained in the latter, attributed to the low loss of the waveguide.
Recently, third harmonic generation has also been demonstrated in plasmonic antennas made of highly doped germanium, allowing the demonstration of a coherent light source tunable between 3 and 5 μm wavelength on Si substrate .
NLO can also been used for wavelength conversion based on four wave mixing. Signal conversion from 2.65 to 1.77 μm was demonstrated using a pump at 2.12 μm in phase matched graded SiGe waveguide .
4.2 Mid-IR monolithically integrated optical modulators and photodetectors
While spectroscopic application would require on-chip modulator for synchronous detection to increase detection sensitivity, most of the works towards Si- and Ge-based optical modulator and photodetectors are developed up to now in the framework of data communication, in the short-wave infrared, i.e. below 4 μm wavelength. Extending the wavelength of data communications towards 2 μm wavelength is envisioned typically for chip-to-chip or board-to-board communications . In this context, the monolithic integration of electro-optic components such as modulator or photodetector is highly required to increase the functionality of the chip.
The field of mid-IR group IV-based optical modulators is still at its infancy. As reported before, Ge-based materials can be used for electro-absorption using Franz-Keldysh in Ge, SiGe or Quantum Confined Stark effect Ge/SiGe QW. These demonstrations have been performed at 1.3–1.5 μm wavelength, the wavelength being determined by the absorption band-edge of the material. Doping Ge with Sn results in a transition from indirect to direct bandgap, but also in a decrease of the bandgap energy. This is the reason why GeSn lasers operate at 2 μm wavelength. Thus the use of GeSn materials has been proposed to achieve light modulation by electro-absorption at this wavelength range. Franz-Keldysh GeSn modulator was designed, with 6 dB extinction ratio for a 2 Vpp drive signal and a 35-GHz bandwidth . It was also proposed to use Quantum Confined Stark Effect in GeSn/SiGeSn QW. Modeling indicates that more than 6 dB extinction ratio should be obtained with a 215-μm long device . To achieve wavelengths beyond 2 μm, alternative effects have to be used. Silicon modulators in the near-IR use free-carrier plasma dispersion effect. The extension of this effect in the MIR has been theoretically evaluated first in Si  and then in Ge . Interestingly, it was predicted that the plasma dispersion effect becomes more effective when the wavelength increases. Experimental demonstrations have then been reported using carrier injection in a silicon PIN diode. Modulation at 2.165 μm has been reported using phase modulation in a Mach-Zehnder interferometer , followed by the demonstration of variable Optical Attenuator at 2–2.5 μm wavelength . Intensity modulation was also demonstrated in the 2-μm band by injecting current through a lateral p-i-n junction in a Ge on Insulator waveguide . Finally, modulators have also been demonstrated working at 3.8 μm wavelength using free-carrier absorption by carrier injection both in a SOI and a Ge-on-Si waveguide .
In parallel with these studies of electro-optic modulation, all-optical modulation has also been demonstrated using free-carrier absorption across wavelength range of 2–3.2 μm .
So far several approaches have been considered for mid-IR on-chip photodetection, most of them relying on heterogeneous integration of III–V material on Si  or other material such as graphene  or nanoparticles . Monolithically integrated Ge-based photodetectors could offer considerable potential for low-cost and high-performance systems. As mentioned earlier, GeSn provides a lower bandgap energy than Ge or SiGe. Photodetection beyond 2 μm was obtained in surface illuminated photodiodes using GeSn/Ge multiple quantum wells , , GeSn-on-Silicon  or Ge/Ge1−xSnx/Ge heterostructures grown on Silicon .
These different approaches related to band-to-band transition are intrinsically limited to SWIR, while there is a need for practical monolithically integrated sensors at longer wavelength. As a good candidate, quantum well infrared photodetectors (QWIPs) rely on intersubband transitions within the QW, thus shorter photon energy is achievable. QWIPs based on SiGe alloys have been demonstrated in different configurations. In initial works, Si-rich structures were considered thanks to the easier procedure for obtaining Si-rich relaxed SiGe virtual substrates . More recently, with the achievement of good quality Ge-rich SiGe virtual substrates , it has been possible to conceive Ge-rich SiGe QW showing intersubband absorption from 6 to 9 μm wavelength at room temperature that can be tuned by adjusting the quantum well thickness .
5 Conclusion and perspectives
Silicon photonics is now a well-established technology. While the use of SOI wafers allows for strong field confinement and tight bends, the combination with Ge permits to obtain high performance active devices required for telecom and datacom applications, at near-IR wavelength. The evolution of Ge-based active devices within Si photonics paved the way towards new wavelength range capabilities, as it allows extending the operation of photonic integrated circuits deep inside the mid-IR range.
Today, wavelengths up to 8.5 μm have been achieved, with propagation loss of only a few dB/cm. A whole set of passive building blocks have also been developed, such as wavelength mulitplexers, fiber couplers or resonators. Main applications are related to absorption spectroscopy, as in this fingerprint wavelength range, most of the molecules have a unique absorption signature, which enables to retrieve and quantify their presence without any waveguide functionalization. First proof of concepts of molecular optical sensing has been demonstrated, based on the absorption of the evanescent tail of the optical mode, or on surface plasmon-enhanced absorption. These works have shown a huge potential for mid-IR absorption spectroscopy.
Active devices such as mid-IR wideband source, modulator and the photodetector are thus required to complete the Ge-based mid-IR platforms. Differents works have already been reported towards this objective, based on a myriad of different physical effects such NLO, plasma dispersion effect, intersubband transitions, Franz-Keldysh or Quantum Confined Stark Effect, to name of few.
Ge-based mid-IR photonics is an exciting and rapidly expanding field. The performance of passive and active devices is continuously improving, and the maximum attainable wavelength range is rapidly expanding. Efforts have been devoted to build basic elements for further complex functionalities within the Ge platform. Interestingly, this evolution relies on the fine comprehension of physical mechanisms of Ge, GeSn and SiGe materials. Based on the current evolution, the use of Ge-based photonics in commercial devices can be expected in a short term.
Financial support is provided by European Research Council (ERC) under the European Union’s Horizon 2020 research and innovation program (N°639107-INsPIRE).
 Reboud V, Gassenq A, Hartmann J-M, et al. Germanium based photonic components toward a full silicon/germanium photonic platform. Prog Cryst Growth Charact Mater 2017;63:1–24.10.1016/j.pcrysgrow.2017.04.004 Search in Google Scholar
 Marris-Morini D, Chaisakul P, Rouifed M-S, et al. Towards low energy consumption integrated photonic circuits based on Ge/SiGe quantum wells. Nanophotonics 2013;2:279–88. Search in Google Scholar
 Mashanovich GZ, Mitchell CJ, Soler Penadés J, et al. Germanium mid-infrared photonic devices. J Light Technol 2016;35:624. Search in Google Scholar
 Zhang L, Agarwal AM, Kimerling LC, Michel J. Nonlinear group IV photonics based on silicon and germanium: from near-infrared to mid-infrared. Nanophotonics 2014;3:247–68. Search in Google Scholar
 Lin H, Luo Z, Gu T, et al. Mid-infrared integrated photonics on silicon: a perspective. Nanophotonics 2018;7:393–420. Search in Google Scholar
 Hartmann J-M, Abbadie A, Papon AM, et al. Reduced pressure-chemical vapor deposition of Ge thick layers on Si(001) for 1.3–1.55 μm photodetection. J Appl Phys 2004;95:5905–13.10.1063/1.1699524 Search in Google Scholar
 Dehlinger G, Koester SJ, Schaub JD, Chu JO, Ouyang QC, Grill A. High-speed germanium-on-SOI lateral PIN photodiodes. J Appl Phys 2004;16:2547–9. Search in Google Scholar
 Klinger S, Berroth M, Kaschel M, Oehme M, Kasper E. Ge-on-Si p-i-n photodiodes with a 3 dB bandwidth of 49 GHz. IEEE Photon Technol Lett 2009;21:920–2.10.1109/LPT.2009.2020510 Search in Google Scholar
 Vivien L, Osmond J, Fédéli JM, et al. 42 GHz p.i.n germanium photodetector integrated in a silicon-on-insulator waveguide. Opt Express 2009;17:6252–7.10.1364/OE.17.006252 Search in Google Scholar
 DeRose CT, Trotter DC, Zortman WA, et al. Ultra compact 45 GHz CMOS compatible germanium waveguide photodiode with low dark current. Opt Express 2011;19:24897–904.2227388310.1364/OE.19.024897 Search in Google Scholar
 Wang J, Loh WY, Chua KT, et al. Low-voltage high-speed (18 GHz/1 V) evanescent-coupled thin-film-Ge lateral PIN photodetectors integrated on Si waveguide. IEEE Photonics Technol Lett 2008;20:1485–7.10.1109/LPT.2008.928087 Search in Google Scholar
 Chen L, Doerr CR, Buhl L, Baeyens Y, Aroca RA. Monolithically integrated 40-wavelength demultiplexer and photodetector array on silicon. IEEE Photonics Technol Lett 2011;23:869–71.10.1109/LPT.2011.2141128 Search in Google Scholar
 Park S, Tsuchizawa T, Watanabe T, et al. Monolithic integration and synchronous operation of germanium photodetectors and silicon variable optical attenuators. Opt Express 2010;18:8412–21.10.1364/OE.18.00841220588687 Search in Google Scholar
 Virot L, Benedikovic D, Szelag B, et al. Integrated waveguide PIN photodiodes exploiting lateral Si/Ge/Si heterojunction. Opt Express 2017;25:19487–96.10.1364/OE.25.01948729041142 Search in Google Scholar
 Baudot C, Douix M, Guerber S, et al. Developments in 300 mm silicon photonics using traditional CMOS fabrication methods and materials; 2017 IEEE International Electron Devices Meeting (IEDM): 1–34. Search in Google Scholar
 Streshinsky M, Ding R, Liu Y, et al. Low power 50 Gb/s silicon traveling wave Mach-Zehnder modulator near 1300 nm. Opt Express 2013;21:30350–7.2451461310.1364/OE.21.030350 Search in Google Scholar
 Marris-Morini D, Baudot C, Fédéli JM, et al. Low loss 40 Gbit/s silicon modulator based on interleaved junctions and fabricated on 300 mm SOI wafers. Opt Express 2013;21:22471–5.2410413610.1364/OE.21.022471 Search in Google Scholar
 Dong P, Liu X, Sethumadhavan C, et al. 224-Gb/s monolithic PDM-16-QAM modulator and receiver based on silicon photonic integrated circuits. Optical Fiber Communication Conference, Anaheim, CA, USA, 2013: PDP5C.6. Search in Google Scholar
 Samani A, Patel D, Chagnon M, et al. Experimental parametric study of 128 Gb/s PAM-4 transmission system using a multielectrode silicon photonic Mach Zehnder modulator. Opt Express 2017;25:13252–62.10.1364/OE.25.013252 Search in Google Scholar
 Milivojevic B, Wiese S, Raabe C, et al. Small-size silicon photonic IQ modulator and low-power CMOS driver for next generation Coherent Transceiver. 18th European Conference on Network and Optical Communications, Graz, Austria, 2013:181–4. Search in Google Scholar
 Shastri A, Muzio C, Webster M, et al. Ultra-low-power single-polarization QAM-16 generation without DAC using a CMOS photonics based segmented modulator. J Light Technol 2015;33:1255–60.10.1109/JLT.2015.2394749 Search in Google Scholar
 Chagnon M, Osman M, Poulin M, et al. Experimental study of 112-Gb/s short reach transmission employing PAM formats and SiP intensity modulator at 1.3 μm. Opt Express 2017;22: 21018–36. Search in Google Scholar
 Xiong C, Gill DM, Proesel JE, Orcutt JS, Haensch W, Green WMJ. Monolithic 56 Gb/s silicon photonic pulse-amplitude modulation transmitter. Optica 2016;3:1060–5.10.1364/OPTICA.3.001060 Search in Google Scholar
 Doerr CR, Chen L, Nielsen T, et al. O, E, S, C and L band silicon photonics coherent modulator/receiver. Optical Fiber Communication Conference Postdeadline Papers, Anaheim, CA USA, 2016:Th5C.4. Search in Google Scholar
 Pérez-Galacho D, Bramerie L, Baudot C, et al. QPSK modulation in the O-band using a single dual-drive Mach-Zehnder silicon modulator. IEEE/OSA J Light Technol 2018;36:3935.10.1109/JLT.2018.2851370 Search in Google Scholar
 Feng NN, Liao S, Feng D, et al. Design and fabrication of 3 μm silicon-on-insulator waveguide integrated Ge electro-absorption modulator. Opt Express 2011;19:8715–20.10.1364/OE.19.008715 Search in Google Scholar
 Schmid M, Kaschel M, Gollhofer M, et al. Franz–Keldysh effect of germanium-on-silicon p–i–n diodes within a wide temperature range. Thin Solid Films 2012;525:110–4.10.1016/j.tsf.2012.10.087 Search in Google Scholar
 Lim AEJ, Liow TY, Qing F, et al. Novel evanescent-coupled germanium electro-absorption modulator featuring monolithic integration with germanium p-i-n photodetector. Opt Express 2011;19:5040–6.10.1364/OE.19.00504021445139 Search in Google Scholar
 Verbist J, Verplaetse M, Srinivasan SA, et al. Real-time 100 Gb/s NRZ and EDB transmission with a GeSi electroabsorption modulator for short-reach optical interconnects. J Light Technol 2018;36:90–6.10.1109/JLT.2017.2775630 Search in Google Scholar
 Verbist J, Lambrecht J, Verplaetse M, et al. DAC-Less and DSP-Free 112 Gb/s PAM-4 transmitter using two parallel electroabsorption modulators. J Light Technol 2018;36:1281–6.10.1109/JLT.2017.2789164 Search in Google Scholar
 Kuo Y, Lee Y, Ge Y, et al. Quantum-confined Stark effect in Ge/SiGe quantum wells on Si for optical modulators. IEEE J Sel Top Quantum Electron 2006;12:1503–13.10.1109/JSTQE.2006.883146 Search in Google Scholar
 Dumas DCS, Gallacher K, Rhead S, et al. Ge/SiGe quantum confined Stark effect electro-absorption modulation with low voltage swing at λ=1550 nm. Opt Express 2014;22: 19284–92.10.1364/OE.22.019284 Search in Google Scholar
 Rouifed MS, Chaisakul P, Marris-Morini D, et al. Quantum-confined stark effect at 1.3 μm in Ge/Si0.35Ge0.65 quantum well structure. Opt Lett 2012;37:3960.10.1364/OL.37.00396023027245 Search in Google Scholar
 Lever L, Hu Y, Myronov M, et al. Modulation of the absorption coefficient at 1.3 um in Ge/SiGe multiple quantum well heterostructures on silicon. Opt Lett 2011;36:4158–60.10.1364/OL.36.004158 Search in Google Scholar
 Chaisakul P, Marris-Morini D, Isella G, et al. Quantum-confined Stark effect measurements in Ge/SiGe quantum-well structures. Opt Lett 2010;35:2913.10.1364/OL.35.00291320808367 Search in Google Scholar
 Ren S, Rong Y, Claussen S, et al. Ge/SiGe quantum well waveguide modulator monolithically integrated with SOI waveguides. IEEE Photonics Technol Lett 2012;24:461–3.10.1109/LPT.2011.2181496 Search in Google Scholar
 Edwards EH, Lever L, Fei E, et al. Low-voltage broad-band electroabsoption from thin Ge/SiGe quantum wells epitaxially grown on silicon. Opt Exp 2013;21:867–76.10.1364/OE.21.000867 Search in Google Scholar
 Rouifed MS, Marris-Morini D, Chaisakul P, et al. Advances toward Ge/SiGe quantum-well waveguide modulators at 1.3 μm. J Sel Top Quantum Electron 2014;20:3400207. Search in Google Scholar
 Vakarin V, Chaisakul P, Frigerio J, et al. Sharp bends and Mach-Zehnder interferometer based on Ge-rich-SiGe waveguides on SiGe graded buffer. Opt Express 2015;23:30821–6.10.1364/OE.23.03082126698715 Search in Google Scholar
 Koerner R, Schwarz D, Clausen C, Oehme M, Fischer IA, Schulze J. The germanium Zenner-emitter for silicon photonics. 19th European Conference on Integrated Photonics, Eindhoven, Netherlands, 2017:M2.2. Search in Google Scholar
 Süess M J, Geiger R, Minamisawa RA, et al. Analysis of enhanced light emission from highly strained germanium microbridges. Nat Photonics 2013;7:466–72.10.1038/nphoton.2013.67 Search in Google Scholar
 Margetis J, Al-Kabi S, Du W, et al. Si-based GeSn lasers with wavelength coverage of 2 to 3 μm and operating temperatures up to 180 K. ACS Photonics 2018;5:827.10.1021/acsphotonics.7b00938 Search in Google Scholar
 Penadés JS, Ortega-Moñux A, Nedeljkovic M, et al. Suspended silicon mid-infrared waveguide devices with subwavelength grating metamaterial cladding. Opt Express 2016;24:22908.10.1364/OE.24.02290827828358 Search in Google Scholar
 Shankar R, Lončar M. Silicon photonic devices for mid-infrared applications. Nanophotonics 2014;3:329–41. Search in Google Scholar
 Hon N K, Soref R, Jalali B. The third-order nonlinear optical coefficients of Si, Ge, and Si1-xGex in the midwave and longwave infrared. J Appl Phys 2011;110:11301.10.1063/1.3592270 Search in Google Scholar
 Chang YC, Paeder V, Hvozdara L, Hartmann JM, Herzig HP. Low-loss germanium strip waveguides on silicon for the mid-infrared. Opt Lett 2012;37:2883.2282516610.1364/OL.37.002883 Search in Google Scholar
 Malik A, Muneeb M, Shimura Y, Van Campenhout J, Loo R, Roelkens G. Germanium-on-silicon planar concave grating wavelength (de)multiplexers in the midinfrared. Appl Phys Lett 2013;103:161119.10.1063/1.4826114 Search in Google Scholar
 Malik A, Muneeb M, Pathak S, et al. Germanium-on-silicon mid-infrared arrayed waveguide grating multiplexers. IEEE Photonics Technol Lett 2013;25:1805.10.1109/LPT.2013.2276479 Search in Google Scholar
 Nedeljkovic M, Penadés JS, Mitchell CJ, et al. Surface-grating-coupled low-loss Ge-on-Si rib waveguides and multimode interferometers. IEEE Photonics Technol Lett 2015;27:1040.10.1109/LPT.2015.2405611 Search in Google Scholar
 Nedeljkovic M, Soler Penades J, Mittal V, et al. Germanium-on-silicon waveguides operating at mid-infrared wavelengths up to 8.5 μm. Opt Express 2017;25:27431.10.1364/OE.25.02743129092216 Search in Google Scholar
 De Leonardis F, Troia B, Passaro VMN. Mid-IR optical and nonlinear properties of germanium on silicon optical waveguides. J Light Technol 2014;32:3747. Search in Google Scholar
 Troia B, Soler Penades J, Khokhar AZ, et al. Germanium-on-silicon Vernier-effect photonic microcavities for the mid-infrared. Opt Lett 2016;41:610.2690743610.1364/OL.41.000610 Search in Google Scholar
 Malik A, Dwivedi S, Van Landschoot L, et al. Ge-on-Si and Ge-on-SOI thermo-optic phase shifters for the mid-infrared. Opt Express 2014;22:28479.10.1364/OE.22.02847925402090 Search in Google Scholar
 Radosavljevic S, Beneitez NT, Katumba A, et al. Mid-infrared Vernier racetrack resonator tunable filter implemented on a germanium on SOI waveguide platform. Opt Mater Express 2018;8:824.10.1364/OME.8.000824 Search in Google Scholar
 Kang J, Takenaka M, Takagi S. Novel Ge waveguide platform on Ge-on-insulator wafer for mid-infrared photonic integrated circuits. Opt Express 2016;24:11855.10.1364/OE.24.01185527410108 Search in Google Scholar
 Alonso-Ramos C, Nedeljkovic M, Benedikovic D, et al. Germanium-on-silicon mid-infrared grating couplers with low-reflectivity inverse taper excitation. Opt Lett 2016;41:4324.10.1364/OL.41.00432427628388 Search in Google Scholar
 Radosavljevic S, Kuyken B, Roelkens G. Efficient 5.2 μm wavelength fiber-to-chip grating couplers for the Ge-on-Si and Ge-on-SOI mid-infrared waveguide platform. Opt Express 2017;25:19034.10.1364/OE.25.019034 Search in Google Scholar
 Kang J, Cheng Z, Zhou W, et al. Focusing subwavelength grating coupler for mid-infrared suspended membrane germanium Waveguides. Opt Lett 2017;42:2094.10.1364/OL.42.00209428569853 Search in Google Scholar
 Sinobad M, Ma P, Luther-Davies B, et al. Dispersion engineered air-clad SiGe waveguides with low propagation loss in the mid-infrared. 2017 Conference on Lasers and Electro-Optics Europe & European Quantum Electronics Conference (CLEO/Europe-EQEC), Munich, Germany; PD-2.5 WED. Search in Google Scholar
 Carletti L, Ma P, Yu Y, et al. Nonlinear optical response of low loss silicon germanium waveguides in the mid-infrared. Opt Express 2015;23:8261.10.1364/OE.23.00826125968664 Search in Google Scholar
 Vakarin V, Ramírez JM, Frigerio J, et al. Ultra-wideband Ge-rich silicon germanium integrated Mach-Zehnder interferometer for mid-infrared spectroscopy. Opt Lett 2017;42:3482–5.10.1364/OL.42.00348228957068 Search in Google Scholar
 Ramirez JM, Vakarin V, Frigerio J, et al. Ge-rich graded-index Si1-xGex waveguides with broadband tight mode confinement and flat anomalous dispersion for nonlinear mid-infrared photonics. Opt Express 2017;25:6561–7.10.1364/OE.25.006561 Search in Google Scholar
 Vakarin V, Ramírez JM, Frigerio J, et al. Wideband Ge-rich SiGe polarization-insensitive waveguides for mid-infrared free-space communications. Appl Sci 2018;8:1154.10.3390/app8071154 Search in Google Scholar
 Liu Q, Ramírez JM, Vakarin V, et al. Mid-IR integrated cavity based on Ge-rich graded SiGe waveguides with lateral Bragg grating. OSA High-brightness Sources and Light-driven Interactions Congress (Mid-Infrared Coherent Sources MICS Strasbourg). Mars 2018. Search in Google Scholar
 Li T, Gao D, Zhang D, Cassan E. High-Q and High-sensitivity one-dimensional photonic crystal slot nanobeam cavity sensors. IEEE Photonics Technol Lett 2016;28:689.10.1109/LPT.2015.2504722 Search in Google Scholar
 Augel L, Berkmann F, Latta D, et al. Optofluidic sensor system with Ge PIN photodetector for CMOS-compatible sensing. Microfluid Nanofluid 2017;21:169.10.1007/s10404-017-2007-3 Search in Google Scholar
 Baldassarre L, Sakat E, Frigerio J, et al. Midinfrared plasmon-enhanced spectroscopy with germanium antennas on silicon substrates. Nano Lett 2015;15:7225−31.2645738710.1021/acs.nanolett.5b03247 Search in Google Scholar
 Gutierrez-Arroyo A, Baudet E, Bodiou L, et al. Optical characterization at 7.7 μm of an integrated platform based on chalcogenide waveguides for sensing applications in the mid-infrared. Opt Express 2016;24:23109–17.10.1364/OE.24.023109 Search in Google Scholar
 Chen Y, Lin H, Hu J, Li M. Heterogeneously integrated silicon photonics for the mid-infrared and spectroscopic sensing. ACS Nano 2014;8:6955–61.2488401310.1021/nn501765k Search in Google Scholar
 Chang YC, Wägli P, Paeder V, et al. Cocaine detection by a mid-infrared waveguide integrated with a microfluidic chip. Lab Chip 2012;12:3020–3.2280614610.1039/c2lc40601b Search in Google Scholar
 Liu Q, Manel Ramirez J, Vakarin V, et al. Mid-infrared sensing between 5.2 and 6.6 μm wavelengths using Ge-rich SiGe waveguides. Opt Mater Express 2018;8:1305.10.1364/OME.8.001305 Search in Google Scholar
 Bettenhausen M, Römer F, Witzigmann B, et al. Germanium plasmon enhanced resonators for label-free terahertz protein sensing. Nanophotonics 2018;72:113–22. Search in Google Scholar
 Frigerio J, Ballabio A, Isella G, et al. Tunability of the dielectric function of heavily doped germanium thin films for mid-infrared plasmonics. Phys Rev B 2016;94:085202.10.1103/PhysRevB.94.085202 Search in Google Scholar
 Frigerio J, Ballabio A, Gallacher K, et al. Optical properties of highly n-doped germanium obtained by in situ doping and laser annealing. J Phys D: Appl Phys 2017;50:465103.10.1088/1361-6463/aa8eca Search in Google Scholar
 Paul DJ, Gallacher K, Millar RW, et al. n-Ge on Si for mid-infrared plasmonic sensors. IEEE Photonics Society Summer Topical Meeting Series (2017) San Juan, Puerto Rico;125–6. Search in Google Scholar
 Augel L, Fischer IA, Hornung F, et al. Ellipsometric characterization of doped Ge0.95Sn0.05 films in the infrared range for plasmonic applications. Opt Lett 2016;41:4398–400.10.1364/OL.41.004398 Search in Google Scholar
 Hon NK, Soref R, Jalali B. The third-order nonlinear optical coefficients of Si, Ge, and Si1-xGex in the midwave and longwave infrared. J Appl Phys 2011;110:011301.10.1063/1.3592270 Search in Google Scholar
 Sohn BU, Monmeyran C, Kimerling LC, Agarwal AM, Tan DTH. Kerr nonlinearity and multi-photon absorption in germanium at mid-infrared wavelengths (2017). Appl Phys Lett 2017;111:091902.10.1063/1.4990590 Search in Google Scholar
 Serna S, Vakarin V, Ramirez JM, et al. Nonlinear properties of Ge-rich Si1-xGex materials with different Ge concentrations. Sci Rep 2017;7:14692.2911620110.1038/s41598-017-15266-z Search in Google Scholar
 Lin Q, Painter OJ, Agrawal GP. Nonlinear optical phenomena in silicon waveguides: modeling and applications. Opt Express 2017;15:16604. Search in Google Scholar
 Yang M, Guo Y, Wang J, et al. Mid-IR supercontinuum generated in low-dispersion Ge-on-Si waveguides pumped by sub-ps pulses. Opt Express 2017;25:16116–22.10.1364/OE.25.01611628789119 Search in Google Scholar
 Ramirez JM, Vakarin V, Frigerio J, et al. Ge-rich graded-index Si1-xGex waveguides with broadband tight mode confinement and flat anomalous dispersion for nonlinear mid-infrared photonics. Opt Express 2017;25:6561.10.1364/OE.25.006561 Search in Google Scholar
 Ettabib MA, Xu L, Bogris A, et al. Broadband telecom to mid-infrared supercontinuum generation in a dispersion-engineered silicon germanium waveguide. Opt Lett 2015;40:4118–21.10.1364/OL.40.004118 Search in Google Scholar
 Sinobad M, Monat C, Luther-Davies B, et al. Mid-infrared octave spanning supercontinuum generation to 8.5 μm in silicon-germanium waveguides. Optica 2018;5:360–6.10.1364/OPTICA.5.000360 Search in Google Scholar
 Fischer MP, Riede A, Gallacher K, et al. Mid infrared nonlinear plasmonics using germanium nanoantennas on silicon substrates. https://arxiv.org/ftp/arxiv/papers/1802/1802.04152.pdf. Search in Google Scholar
 Hammani K, Ettabib MA, Bogris A, et al. Towards nonlinear conversion from mid- to near-infrared wavelengths using silicon germanium waveguides. Opt Express 2014;22:9673. Search in Google Scholar
 Ponce R, Sharif Azadeh S, Stange D, et al. Design of a high-speed germanium-tin absorption modulator at mid-infrared wavelengths. Proc IEEE Conf Group IV Photonics (GFP), Berlin, Germany, 2017:19–20. Search in Google Scholar
 Akie M, Fujisawa T, Sato T, Arai M, Saitoh K. GeSn/SiGeSn multiple-quantum-well electroabsorption modulator with taper coupler for mid-infrared Ge-on-Si platform. IEEE J Sel Top Quantum Electron 2018;24:3400208. Search in Google Scholar
 Nedeljkovic M, Soref R, Mashanovich GZ. Free-carrier electrorefraction and electroabsorption modulation predictions for silicon over the 1–14-μm infrared wavelength range. IEEE Photonics J 2011;3:1171.10.1109/JPHOT.2011.2171930 Search in Google Scholar
 Nedeljkovic M, Soref R, Mashanovich GZ. Predictions of free-carrier electroabsorption and electrorefraction in germanium. IEEE Photonics J 2015;7:2600214. Search in Google Scholar
 Van Camp MA, Assefa S, Gill DM, et al. Demonstration of electrooptic modulation at 2165 nm using a silicon Mach-Zehnder interferometer. Opt Express 2012;20:28009.10.1364/OE.20.028009 Search in Google Scholar
 Shen L, Healy N, Mitchell CJ, et al. Mid-infrared all-optical modulation in low-loss germanium-on-silicon waveguides. Opt Lett 2015;40:268–71.2567986110.1364/OL.40.000268 Search in Google Scholar
 Muneeb M, Vasiliev A, Ruocco A, et al. III-V-on-silicon integrated micro-spectrometer for the 3 μm wavelength range. Opt Express 2016;24:9465–72.2713756010.1364/OE.24.009465 Search in Google Scholar
 Roelkens G, Dave UD, Gassenq A, et al. Silicon-based photonic integration beyond the telecommunication wavelength range. IEEE J Sel Top Quantum Electron 2014;20:8201511. Search in Google Scholar
 Gassenq A, Gencarelli F, Van Campenhout J, et al. GeSn/Ge heterostructure short-wave infrared photodetectors on silicon. Opt Express 2012;20:27297.10.1364/OE.20.02729723262679 Search in Google Scholar
 Cong H, Xue C, Zheng J, et al. Silicon based GeSn p-i-n photodetector for SWIR detection. IEEE Photonics J 2016;8:6804706. Search in Google Scholar
 Pham T, Du W, Tran H, et al. Systematic study of Si-based GeSn photodiodes with 2.6 μm detector cutoff for short-wave infrared detection. Opt Express 2016;24:4519.10.1364/OE.24.004519 Search in Google Scholar
 Gallacher K, Ballabio A, Millar RW, et al. Mid-infrared intersubband absorption from p-Ge quantum wells grown on Si substrates. Appl Phys Lett 2016;108:091114.10.1063/1.4943145 Search in Google Scholar
©2018 Delphine Marris-Morini et al., published by De Gruyter, Berlin/Boston
This work is licensed under the Creative Commons Attribution-NonCommercial-NoDerivatives 4.0 License.